Phase Change Materials in Floor Tiles for Thermal
Phase Change Materials in Floor Tiles for Thermal Energy Storage
October 2000 - August 2002
Submitted by: Douglas C. Hittle
Award No. DE-FC26-00NT40999
Colorado State University
Fort Collins, CO 80523
“This report was prepared as an account of work sponsored by an agency of the United States
Government. Neither the United States Government nor any agency thereof, nor any of their
employees, makes any warranty, express or implied, or assumes any legal liability or
responsibility for the accuracy, completeness, or usefulness of any information, apparatus,
product, or process disclosed, or represents that its use would not infringe privately owned rights.
Reference herein to any specific commercial product, process, or service by trade name,
trademark, manufacturer, or otherwise does not necessarily constitute or imply its endorsement,
recommendation, or favoring by the United States Government or any agency thereof. The
views and opinions of authors expressed herein do not necessarily state or reflect those of the
United States Government or any agency thereof.”
Passive solar systems integrated into residential structures significantly reduce heating energy
consumption. Taking advantage of latent heat storage has further increased energy savings. This
is accomplished by the incorporation of phase change materials into building materials used in
passive applications. Trombe walls, ceilings and floors can all be enhanced with phase change
materials. Increasing the thermal storage of floor tile by the addition of encapsulated paraffin
wax is the proposed topic of research.
Latent heat storage of a phase change material (PCM) is obtained during a change in phase.
Typical materials use the latent heat released when the material changes from a liquid to a solid.
Paraffin wax and salt hydrates are examples of such materials. Other PCMs that have been
recently investigated undergo a phase transition from one solid form to another. During this
process they will release heat. These are known as solid-state phase change materials. All have
large latent heats, which makes them ideal for passive solar applications. Easy incorporation into
various building materials is must for these materials. This proposal will address the advantages
and disadvantages of using these materials in floor tile.
Prototype tile will be made from a mixture of quartz, binder and phase change material. The
thermal and structural properties of the prototype tiles will be tested fully. It is expected that
with the addition of the phase change material the structural properties will be compromised to
some extent. The ratio of phase change material in the tile will have to be varied to determine
the best mixture to provide significant thermal storage, while maintaining structural properties
that meet the industry standards for floor tile.
TABLE OF CONTENTS
Introduction . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . .
Executive Summary. . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . .
Phase Change Materials . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . .
Phase Change Material Candidates . . . . . . . . . . . . . . . . . . . . . . . . . . . .
Salt Hydrates. . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . .
Solid-State Phase Change Materials. . . . . . . . . . . . . . . . . . . . . . . . . . . .
Layered Perovskites. . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . .
Plastic Crystals. . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . .
Background on Plastic Crystals . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . .
Paraffin Wax. . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . .
Outlast Technology . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . .
Experiments . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . .
Comparison of Thermal Properties of Phase Change Materials . . . . . .
Under Cooling Effects of Phase Change Materials . . . . . . . . . . . . . . . .
Potential Energy Storage Capabilities of Phase Change Materials . . . .
Binders . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . .
Binder for Solid-State Phase Change Materials. . . . . . . . . . . . . . . . . . .
Binder for Paraffin Wax. . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . .
Cost Analysis of Components. . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . .
Structural Integrity of Encapsulated Particles. . . . . . . . . . . . . . . . . . . .
Final Material Selection. . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . .
Phase Change Material. . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . .
Binder . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . .
Potential Energy Saving Analysis. . . . . . . . . . . . . . . . . . . . . . . . . . . . .
Expected Solar Gain. . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . .
Solar Load Ratio Calculation. . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . .
Possible Annual Savings . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . .
Future Simulations. . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . .
Tile Mixture . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . .
Varying Binder Proportions. . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . .
Addition of Phase Change Material. . . . . . . . . . . . . . . . . . . . . . . . . . . .
Prototype Testing Research . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . .
Physical Testing . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . .
Initial Testing. . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . .
Thermal Testing. . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . .
Prototype Manufacture. . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . .
Results and Discussion. . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . .
Preliminary Compression Testing . . . . . . . . . . . . . . . . . . . . . . . . . . . .
Preliminary Thermal Testing Results. . . . . . . . . . . . . . . . . . . . . . . . . . .
Conclusion. . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . .
References. . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . .
Appendix 1. . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . .
Appendix 2. . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . .
Appendix 3. . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . .
Appendix 4. . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . .
LIST OF FIGURES
Phase of a: I. liquid crystal II. typical crystal III. plastic crystal
Sample tile with resin mass fraction of 8% (No phase change material)
Sample tile with resin mass fraction of 12% (No phase change material)
Sample tile with phase change material incorporated with
Sample time with phase change material incorporated without
4" Tile mold
Tile mold in press
Molecular structure of pentaerythritol, C – (CH2OH)4
Molecular structure of pentaglycerine, (CH3) – C – (CH2OH)3
Molecular structure of neopentyl glycol, (CH3)2 – C – (CH2OH)2
Latent Heat for Binary Mixture of Neopentyl Glycol
Molecular Structure of Melamine-Formaldehyde
LIST OF TABLES
Thermal Properties of Phase Change Materials
Under Cooling for DSC Measurements Taken at 5oC/min
Potential Energy Storage of 100% Phase Change Floor Tile
Potential Energy Storage Adjusting for Encapsulation Shell
Binder Approximate Costs
Final and Bulk Cost of Phase Change Materials
Estimated Monthly Absorbed Solar Radition per Area of South Glazing
Potential Energy Storage for a Floor Area of 346.5 ft2
Absorbed Average Daily Radiation through South Glazing of
Area 352 ft2
Coefficients used for NLC Calculation
Dimensions of Passive Reference Design
Increase in Solar Saving from Basic Reference Design
Annual Heating Cost Savings
Granirex Recipe Proportions
Selected Physical Tests
Preliminary DSC Testing
Kenwax 18 Paraffin Content
Kenwax 19 Paraffin Content
Physical Tests Performed on Agglomerate Floor Tile by
The use of solar energy to offset fuel consumption in commercial and residential buildings can
be accomplished by implementing active or passive solar systems. Duffie and Beckman14 give
the following basic distinction of these two systems. Active solar systems include the use of
collectors and storage systems that are not integrated with the building structure, while passive
systems are integrated within the building structure. The proposed research is concerned with
increasing the efficiency of passive solar applications by enhancing the thermal mass. Thermal
storage capacity of floor tile will be increased with the addition of phase change materials.
Traditional passive design involves the addition of a sunspace to a structure. The purpose of this
room is to store thermal energy and then subsequently release the energy to aid in the reduction
of the heating load. Energy is gained directly from the sun through the glazing in the sunspace,
with the majority entering through the south-facing windows. The south-facing wall should
contain 0.19 to 0.3814 glazing area to floor area in order to maximize energy collected.
Floors and walls traditionally make up the thermal mass of a sunspace. Typically construction
materials are concrete, masonry brick or dark clay tile. Thermal storage is usually accomplished
by sensible heat storage. Heat is stored as the material temperature increases due to the solar
energy entering the space. As a result, the space can easily become overheated. Solutions to
prevent overheating can be accomplished in several ways. The south-facing glazing area can be
decreased or an overhang can be placed over the south facing glazing to reduce the amount of
direct sunlight entering the space during the summer months. Installation of fans for increased
ventilation and circulation can also aid in reducing overheating. Another solution is to
incorporate latent heat storage.
Heat is released during a change in phase of a material. All materials undergo phase transitions,
thus have an associated latent heat. When a substance melts, vaporizes and sublimates, heat is
absorbed. Heat is released when a material solidifies and condenses. During a change in phase,
the temperature remains practically constant.
Since the temperature stays virtually constant during a change in phase, the temperatures of the
thermal mass are lower. Lower temperatures mean less heat loss and a comfortable room
temperature even during the summer months. It also results in a more consistent room
temperature and reduction in overheating. Another advantage of latent heat storage is greater
volumetric energy storage compared to sensible heat storage.
Phase change materials can be incorporated into building materials used in passive applications.
Wood, gypsum board, lightweight concrete and floor and ceiling tile can all be enhanced with
the addition of phase change materials. The ceiling, floor and walls are all large surface areas in
a sunspace that are perfect candidates for latent heat storage.
2. EXECUTIVE SUMMARY
We refresh the reader by describing the technology that we hope to license to manufacturers of
agglomerate floor tile.
One of the standard agglomerate floor tiles manufactured today consists of quart chips, quartz
powder (filler), dyes, and a polyester binder. Components are mixed in what looks like a giant
cement mixer. The mix, appearing and feeling much like damp sand, is placed in a vibrating
vacuum assembly to remove all air and to compress the material. Next, the slabs of material are
heated to cause catalysis. Later, slabs are cut and polished to produce the desired tiles.
Our proposal is to substitute micro encapsulated phase change material for much, if not all of the
quartz power used in the recipe above. We may also be able to replace some of the chips without
degrading the tile appearance. We will refer to this tile as PCM floor tile, hereinafter.
Putting phase change material in the floor tile dramatically increases its ability to store thermal
energy. Also, the energy is stored at a nearly constant temperature. One application is the use of
the tile in sunroom floors where it can absorb solar energy during the day and release it at night
to reduce mechanical heating. The resultant reduced heating bills need to be sufficient to offset
any additional first costs associated with the use of the phase change floor tiles.
Because agglomerate floor tiles have exceptional wear resistance properties, they are often
marketed to institutional clients that have high traffic areas. Just as professional basketball teams
may “have a foul to give,” the residential applications we have in mind (sun rooms or other areas
that receive direct sunlight) do not have the traffic of say, an airport concourse. Our challenge
then is to maximize the amount of phase change material used in the floor tile without ruining
the tile’s physical properties. We have “wear properties to give” compared to agglomerate floor
tiles because we expect the tiles to be used in less demanding applications.
To date, we have made floor tile samples that contain PCM as a substitute for the quartz filler.
These tiles have structural properties that are not quite as good as agglomerate tiles without
PCMs, but are significantly better than fired clay tiles often used in residential applications. We
have explored variations in tile composition of the tile and how they affect tile structural
properties. We have also made preliminary contact with prospective licensees and are
participating in DOE’s Commercialization Program.
3. PHASE CHANGE MATERIALS
All materials have an associated latent heat for each phase change, but only a few are appropriate
for passive solar applications. They need to have a reversible transition, a high latent heat, and
small changes in volume between phases and low vapor pressure. They must be chemically
stable and good heat conductors. These properties also have to occur at the appropriate transition
temperature. Depending on the passive application, the required transition temperature will vary.
However, for a sunspace it needs to be approximately 27oC(80oF). The transition temperature is
crucial to attaining the maximum heat storage during the day and maximum heat release at night.
During the heating season, the nights are longer than the daylight hours. The optimal transition
temperature is one-third of the way between the lowest tolerable temperature and the highest
tolerable temperature of the space.38
3.1 Phase Change Material Candidates
Traditional phase change materials that have been studied and used in applications are alkanes,
paraffin waxes and salt hydrates. These materials undergo a reversible solid to liquid phase
change at various transition temperatures. Studies have been performed for the feasibility of
using solid-state phase change materials for latent heat storage. The biggest advantage the solidstate phase change materials have is no liquid phase to contain—the materials change from
amorphous to crystalline phases while remaining “solid.” Both paraffin wax and salt hydrates
usually have to be encapsulated to contain the liquid phase, which adds to the final cost of the
Paraffin wax and salt hydrates have been successfully incorporated into building materials such
as wallboard and concrete. A few products have been marketed commercially. Incorporation of
solid-state phase change material in concrete has been accomplished in laboratory settings.
Sheets of the solid-state phase change materials have also been used as flooring for a research
simulation of the effect of latent heat storage in flooring.
The candidate building product that we are considering is floor tile. Phase change floor tile can
be used in sun spaces to store energy from the sun during the day while releasing it during the
Salt hydrates are inorganic materials. Inorganic compounds have twice the volumetric latent
energy storage compared to organic compounds. The organic compounds however, have the
advantages of melting congruently, self-nucleation and are non-corrosive.25 Salt hydrates will
melt incongruently causing phase separation.
Naumann37 reported that the incongruent melting behavior of Glauber salts results in two or three
different solidification steps upon cooling below the melting temperature. This was observed at
20 degrees below the melting temperature. The application of nucleating agents reduced this
effect to one degree.
3.2 Salt Hydrates
These materials were not considered a candidate for floor tile for several reasons. If a container
is required to contain the liquid phase, metal containers cannot be used because the salt hydrates
are corrosive. Crystallization of the salts can also lead to tears forming in polymer containers.
They are also known to form partially hydrated or less soluble crystals due to the high rates of
crystallization of the subcooled melts.6 These less soluble crystals undergo phase transitions at
much higher temperatures, thus lowering the thermal storage capabilities over time.
3.3 Solid-State Phase Change Materials
Materials that undergo an additional phase transition between the solid and liquid state belong to
a group of solid-state phase change materials. A transition occurs from one solid state to
another. This transition is associated with large latent heats of transformation. Additional
advantages are, usage significantly below melting temperatures requiring very little or no
containment and easy incorporation in building materials. There are two categories of solid-state
phase change materials, layered perovskites and plastic crystals.
3.3.1 Layered Perovskites
Layered perovskites are chemical compounds with the general formula of:
(n-Cn H2n+1 NH3)2MCL4
is a divalent metal atom such as Mn, Cu, Hg or Fe.
8 ≤ n ≤ 18
The structure is composed of regular alteration of inorganic and hydrocarbon regions. Each
inorganic layer is sandwiched between two hydrocarbon layers. The hydrocarbon regions are
composed of long chain alkylammonium groups ionicly bonded to the inorganic support.9 These
linear alkyl chains are responsible for thermal behavior of the material.
At low temperatures the alkyl chains are in an ordered planar zigzag arrangement. The chains
are in a disordered state at high temperatures. They exhibit “liquid-like” behavior in this state.
A liquid phase is not obtained at this point because the alkyl chains are fixed on one end to the
inorganic layer, thus keeping its lattice structure.9
One advantage is that transition temperatures are dependent on alkyl chain length so control of
transition temperatures can be accomplished. Other advantages are a relatively high thermal
conductivity and chemical stability at high temperatures.8 Disadvantages are possible toxicity,
lower value of enthalpy per unit cost and the total latent heat is reduced due to the inorganic
regions of the molecules that are inert.9
3.3.2 Plastic Crystals
NASA studied a group of solid-state materials during the 1970’s for passive temperature control
of earth satellites.7 Three materials were shown to be promising for passive applications:
pentaerythritol (PE), pentaglycerine (PG) and neopentyl glycol (NPG).
These materials belong to a class of compounds called polyalcohols or polyols. Each molecule
has a central carbon atom with four attached carbon atoms forming a tetrahedron. The number
of hydroxyl groups attached to the four carbon atoms distinguished the three compounds from
each other.45 Pentaerythritol is the largest molecule, the smallest is neopentyl glycol. Molecular
structures of these materials are presented in Appendix 1 in Figures 8-10.
The most stable form of these materials is a crystalline solid. As heat is applied the material
undergoes a transition to a plastic crystal. This behavior comes from the tetrahedral molecular
shape and the hydrogen resonant bonding that occurs between neighboring molecules.6 The
substance will eventually melt as the temperature is further increased and will eventually turn
into a gas. It is the transition from crystalline solid to a plastic crystal that is of interest.
3.3.3 Background on Plastic Crystals
Plastic crystals are defined as a type of mesophase. The term mesophase, shortened from
mesomorphic, was introduced by Friedel in 1922.23 He defined it as a phase with microscopic
structures between solids and ordinary isotropic liquids. He stated that there were two distinct
types of this phase, which he described as smectic and nematic. Earlier, the term “liquid crystal”
was used to describe both these phases. Otto Lehmann coined the phrase “liquid crystal” in
1889. The actual discovery of this phase is attributed to an Austrian botanist, Friedrich
Reinitzed, in 1888.23 Friedel did not agree with the term “liquid crystal” which lead to his use of
smectic and nematic to describe two types of this phase.
In 1935, Timmermans recognized a third type of mesophase, “plastic crystals”. Later,
Wunderlich and Grebowitz further distinguished three types of mesophases referred to as liquid
crystals, plastic crystals and condis. Condis is often confused with liquid crystals since they are
similar in nature.8 All three types exhibit some degree of long-range order similar to crystals.
They also show a degree of mobility other than segment vibrations, which is similar to isotropic
liquids.8 This is why the term “liquid crystal” was first used to describe this phase.
The difference between these three types of mesophases are the types of disordering they
display. Liquid crystals exhibit a positional disordering. Plastic crystals show positional
disordering but also display orientational disordering. The final type, condis, displays
conformational disordering as well as positional and orientational disordering.8 In positional
disordering, the intermolecular distances become less uniform and the molecules can arrange
themselves parallel, perpendicular or randomly. Conformational disordering is the acquisition of
freedom of executing rotations about single bonds.35
A further distinction between liquid and plastic crystals can been seen in Figure 1. In this figure,
the phases are given for liquid, plastic and ordinary crystals. A typical crystal on increasing
temperature will transform directly into the liquid state. This is shown by Case II in Figure 1.
Both liquefaction and isotropy occur at the same temperature. This is not true of plastic and
liquid crystals. Liquid crystals first undergo liquefaction then become isotropic. The opposite is
true of plastic crystals were isotropy occurs first. Case I and III both show the behavior of liquid
and plastic crystals respectively. This figure was taken from Timmermans.45
3.4 Paraffin Wax
Normal paraffin waxes are part of a family of saturated hydrocarbons. The structure is the type
CnH2n+2. Those with carbon atoms between five and fifteen are liquids at room temperatures and
are not considered. Normal or straight chain and symmetrically branched chain paraffin waxes
are the most stable. Typically, paraffin waxes with odd numbers of carbon atoms are more
widely used because they are more available, more economical and have higher heats of fusion.
Figure 1. Phase of a: I. liquid crystal II. typical crystal III. plastic crystal
Paraffin waxes are composed mainly of alkanes, approximately 75%.25 Alkanes and paraffin
waxes are both organic compounds. Paraffin can contain several alkanes resulting in a melting
range rather than a melting point. As the molecular weight increases, the melting point tends to
increase as well. Using different mixtures of alkanes, specific transition temperatures for
paraffin waxes can be attained. Paraffin waxes and alkanes at the transition temperature melt to
a liquid and solidify upon cooling. They do not have the containment problems of salt hydrates.
The only requirement is a flexible containment to allow for the small volume change from the
The properties of normal paraffin wax are very suitable for latent heat storage. They have a large
heat of fusion per unit weight, non-corrosive, nontoxic, chemically inert and stable below 500oC
(932oF). On melting, they have a low volume change and a low vapor pressure. Mixing
different molecular weight paraffin waxes together can easily vary melting temperature. Since
they are commercially available, the cost is reasonable. Prime candidates for passive
applications are tetradecane, hexadecane, octadecane and eicosane. Paraffin wax, as well as
solid-state phase change materials, has a low thermal conductivity. However, the addition of
additives such as graphite could increase the thermal conductivity.6
3.4.1 Outlast Technology
A Boulder, Colorado company, Outlast Technology, is incorporating encapsulated paraffin wax
into fabric for outerwear using a technology originally developed for NASA. The technology
involves the microencapsulation of microscopic size droplets of paraffin wax. These
encapsulated particles of wax are then incorporated into fabrics and foams that are used for
Outlast currently uses two grades of phase change materials in order to fit to different
applications. One application is for cold weather/extremity wear designed to operate from
18.3oC to 29.4oC (65oF to 85oF). The other grade is used in four season applications designed to
operate from 26.7oC to 37.8oC (80oF to 100oF).33 The grades are composed of a mixture of
paraffin waxes from a carbon count of 15 to 24. A mixture is used in order to cut production
costs. Pure forms of paraffin waxes are significantly more expensive due to the refining
Capsules are on the order of 21µm.
Using this process of
microencapsulation and the appropriate mixture of paraffin, a suitable candidate can be found for
the floor tile application.
4.1 Comparison of Thermal Properties of Phase Change Materials
Paraffin wax and solid-state phase change materials have transition temperatures and heats of
fusion suitable for passive solar applications. A transition temperature around room temperature,
80oF (27oC) is ideal. Thermal properties of these materials are presented in Table 1.
Table 1. Thermal Properties of Phase Change Materials
Heat of Fusion
269 J/g (115 Btu/lbm)
139 J/g (59.8 Btu/lbm)
Neopentyl Glycol (NPG)
119 J/g (51.2 Btu/lbm)
60%NPG and 40%PG
76 J/g (32.7 Btu/lbm)
228 J/g (98 Btu/lbm)
237 J/g (102 Btu/lbm)
244 J/g (105 Btu/lbm)
244 J/g (105 Btu/lbm)
165 J/g (71 Btu/lbm)
151 J/g (65 Btu/lbm)
The transition temperature of the solid-state phase change materials in the pure form is not low
enough for use in passive applications. By mixing these compounds in various ratios, the
transition temperature can be lowered. The ideal ratio was determined to be a mixture of 60%
neopentyl glycol and 40% pentaglycerine. Both Benson4,6 and Font18 have presented this ratio in
their research. It also has been repeated in the laboratory during early research for this project.
Benson6 reported the number of intermolecular hydrogen bonds largely controls the amount of
energy absorbed at transition. Altering the number of hydrogen bonds can have a significant
effect on the energy absorbed and the transition temperature. This can be accomplished by
mixing the pure forms of the solid-state materials with each other. The materials readily form
binary mixture with each other either by dissolution in water or in their molten forms.
Pure octadecane is very close to the defined ideal passive temperature. Outlast uses mixtures of
normal paraffin wax, Kenwax 18 and 19, for the phase change material. The paraffin content of
these two mixtures is listed in Appendix 2. By mixing normal alkanes of different molecule
weights, the melting or transition temperature can be altered from that of the pure form.
One obvious effect of mixing phase change materials is that the latent heat is lowered. The
mixture of 60% NPG and 40% PG, as presented in Table 1, results in more than 50% decrease
in the latent heat storage capabilities. Kenwax mixtures experience a decrease, although not as
drastic. Outlast determined that the latent heat of a blend can be found from a linear equation,
Final Blend J/g = (wt.% mPCM1 x J/g mPCM1) + (wt.% mPCM2 x J/g mPCM2) + …
Studies performed by Benson6 and Font21 did not show a linear relationship between the molar
percentage of neopentyl glycol and pentaglycerine, and latent heat. The latent heat decreases
from the pure form of pentaglycerine as neopentyl glycol was added until the mixture contained
60% NPG. At that mixture, the latent heat, as well as the transition temperature, began to
increase to the latent heat for the pure form of neopentyl glycol. Results of analysis done by
Benson and Font are presented in Appendix 1.
Octadecane in its pure form has the highest heat of fusion with a transition temperature close to
the ideal passive temperature. Its latent heat storage is more than three times greater than the
NPG/PG mixture. Based on thermal storage capabilities, octadecane is the superior material,
followed by the Kenwax 18.
4.2 Under Cooling Effects of Phase Change Materials
Paraffin wax and solid-state phase change materials show the behavior of under or super cooling.
This behavior occurs when the material does not solidify at the same temperature at which it
melted. Solid-state phase materials have shown more than a twenty-degree difference. The
difference is not as noticeable in paraffin waxes.
Measurements have been made using a differential scanning calorimeter (DSC) to show the
undercooking effect. The DSC is an apparatus that controls the cooling and heating of a
material. Materials were heated at 5oC per minute beyond the transition temperature and then
allowed to cool at the same rate. The difference between the transition temperature during
heating and cooling is presented in Table 2. Measurements were taken for the solid-state phase
change material by Benson, and Outlast took measurements for Kenwax 18 and 19.
Nucleating agents, such as powder graphite, can be also added to help further reduce under
cooling. Benson6 showed the addition of 0.1%-powdered graphite aided in the reduction of
Table 2. Under Cooling for DSC Measurements Taken at 5oC/min
60%NPG and 40%PG
∆T Between Heating
Studies by Yamagishi48 presented the result of the use of derivatives of n-paraffin waxes to
cancel under cooling effects. 1-Tetradecanol was selected as the nucleating agent for
tetradecane. Results showed a 2% addition of the nucleating agent canceled the undercooking
Further analysis by Yamagishi48 found the size of an encapsulated particle of paraffin to affect
the degree of under cooling. As the size of the particle is decreased the crystallization
temperature decreases, thus increasing the degree of under cooling. This is due to the fact that as
the size decreases, the number of nuclei to start crystallization in each particle decreases.
Particles from the range of 100-to1000 µm show a constant difference of approximately 10oC
between melting and crystallization temperatures. However, particles in the range of 5 to 100
µm had a drop from a 10oC difference to a more than 20oC difference. Again the addition of
nucleating agents can reduce this difference.
4.3 Potential Energy Storage Capabilities of Phase Change Materials
Based on the latent heat and the density of the phase change materials, the potential energy
storage can be calculated. Assuming a floor tile composed of 100% phase change material, the
energy storage per square area is presented in Table 3. Two common thicknesses of tiles were
used for the analysis.
Results presented in Table 3 shows octadecane to have twice the potential energy storage of the
solid-state phase change mixture. Kenwax 18 has one and one half times more potential energy
storage over the solid-state mixture. As expected, the thicker tile has the greater heat storage and
would be the best selection for the floor tile.
It should be mentioned that the potential energy storage of Kenwax and octadecane does not
include the encapsulation material. The microencapsulation shell is approximately one micron
thick with the core taking 80-85% of the weight.11 Results from Table 4 should be reduced to
account for the encapsulation shell.
Table 3. Potential Energy Storage of 100% Phase Change Floor Tile
½” Floor Tile
1.08 MJ/m2 (95.6 Btu/ft2)
1.60 MJ/m2 (141.4 Btu/ft2)
2.52 MJ/m2 (222.3 Btu/ft2)
¾” Floor Tile
1.63 MJ/m2 (143.5 Btu/ft2)
2.40 MJ/m2 (212.1 Btu/ft2)
3.78 MJ/m2 (333.4 Btu/ft2)
Table 4 shows the effect of an 80% to 85% reduction. Octadecane still has a storage potential
approximately twice as great as the solid-state phase change mixture. The effect on the Kenwax
18 is more noticeable. Its energy storage potential is still larger, but is more on the scale of the
solid-state phase change mixture. The preferred phase change material based on the potential
energy storage is octadecane.
Table 4. Potential Energy Storage Adjusting for Encapsulation Shell
½” Floor Tile
1.28 - 1.36 MJ/m2
2.02 – 2.14 MJ/m2
¾” Floor Tile
1.92 – 2.04 MJ/m2
3.02 – 3.21 MJ/m2
Potential energy storage is a theoretical value and not obtainable in real floor tile. It can be
assumed that in an actual floor tile the phase change materials would only occupy, at best, 50%
of the total tile. The remainder of the tile is composed of the binder and agglomerate, such as
quartz. However, the optimum potential energy does provide a useful gauge in the benefit of
using one type of phase change material over another. Based on potential energy storage the
phase change with the largest latent heat storage would be the best choice.
The focus of this research is to incorporate a phase change material into an agglomerate floor
tile. Prototype tiles will have three main components. A binder, phase change material and a
combination of quartz rock chips and quartz powder. The quartz rock and powder are for
strength and appearance. The type of binder will depend on the phase change material used for
4.4.1 Binder for Solid-State Phase Change Materials
Initially unsaturated polyester, with styrene as a liquid monomer, was used as the binder.
However, the tile mixture would not cure when the solid-state phase change material was added.
It was assumed the phase change material was preventing the cure.
Polyesters use carboxylic acids and polyfunctional alcohols like neopentyl glycol, to impart
flexibility, toughness and stain and chemical resistance. Neopentyl glycol is often used in the
polyester synthesis for improved stain and chemical resistance. Propylene glycol is typically
used with the unsaturated monomer styrene. It is believed that with the addition of neopentyl
glycol and pentaglycerine, cross-linking was being prevented.
Epoxies were then investigated as possible binders for solid-state phase change materials. An
epoxy resin and curing agent produced by Shell Chemicals was the second binder tested. EPON
828 and curing agent 3140 was combined with the phase change materials and quartz. This
mixture did cure to form a piece of prototype tile. The amount of phase change material was
small, but DSC runs did show a phase transition at the appropriate transition temperature.
EPON 828 is an undiluted clear difunctional bisphenolA/epichlorohydrin derived liquid epoxy
resin.16 This material is cross-linked with an appropriate curing agent to form a material with
good adhesive, mechanical, dielectric and chemical resistance properties. The curing agent
3140 is a low viscosity reactive polyamide and high imidazoline, which is based on dimerized
fatty acid and polyamines.15
Solid-state phase change materials have also been shown to react adversely with the epoxy resin.
The solid-state materials, NPG, PG, PE and the 60/40 NPG/PG mixture all have available
hydroxyl groups to react with epoxy groups. The solid-state phase change material was causing
the rate of cross-linking to increase by acting like a curing agent. This resulted in a decrease in
the thermal storage capability of the phase change material, since some of phase change material
was being used during the cure.
4.4.2 Binder for Paraffin Wax
It is expected that paraffin wax will not react adversely with epoxies or polyesters. The material
used for the encapsulation is relatively inert. Encapsulation of melamine resin was determined
by Yamagishi48 not to react with the brine solutions CaCl2, NaCl, glycol or silicon oil. Outlast
Technology uses melamine-formaldehyde as the encapsulation material and found it was durable
and did not react adversely with other materials.
Melamine-formaldehyde resin belongs to the family of thermosets. The high cross-linking
nature of the cure product results in superior hardness, strength and rigidity. High chemical and
abrasion resistance are other strong attributes of the material. It is widely used in decorative
laminate such as Formica. The molecular structure is given in Appendix 3. Sites can remain
active if cross-linking is not complete, which may react with the tile binder. However it is not
seen as a risk, as the encapsulation process is expected to be a complete cure.
4.5 Cost Analysis of Components
An area for concern is the final cost of the floor tile. The type of binder and phase change
material used effects final costs. It is assumed that the amount of quartz rock and powder would
be the same regardless of binder and phase change material used. The type of binder will depend
on the phase change material selected. Solid-state phase change material requires an epoxy to be
used, while polyesters can be used with encapsulated paraffin particles. Table 5 shows that the
costs of general-purpose polyesters are half the cost of epoxies.
Table 5. Binder Approximate Costs
Shell EPI_CURe 3140
Shell EPI-CURe 3234
Shell Resin 828
Ashland chlorendic polyester HETRON 197-3
Ashland isophthalic polyester AROPOL 7241
$1.30 to $1.50 / lb
$2.00 to $4.00 / lb
$1.65 / lb
$1.65 / lb
$1.65 / lb
$0.65 to $0.70 / lb
$1.81 / lb
$1.44 / lb
Bulk costs of the phase change materials depend on the current commercial use of the materials.
Neopentyl glycol is used in paint and resin production, which reduces the cost of the raw
product. However pentaglycerine is not as widely used and will increase the final cost of the
solid-state phase change mixture significantly.
Paraffin waxes are widely used in many different applications and can be obtained in many
different grades. The level of processing assigns grades. A pure form of octadecane, 99%, is
more expensive than the 97% form. Kenwax used by Outlast is a mixture of paraffin waxes and
does not undergo as much refinement, so the cost is even less. However a decrease in the latent
heat storage is accompanied with the use of unrefined paraffin, as values in Table 1 show.
Encapsulation processing for the paraffin wax makes up most of the final costs as seen in Table
6. The table also shows the bulk costs of the raw phase change materials.
Table 6. Final and Bulk Cost of Phase Change Materials
Solid-State Phase Change Materials
Outlast Kenwax 18 and Kenwax 19
Technical Grade Octadecane (~95%)
Encapsulation Final Costs
Outlast Kenwax 18 and Kenwax 19
Technical Grade Octadecane (~95%)
$0.74 / lb
$0.67 / lb
$9 - $12 /lb
The final costs of the encapsulated paraffin and solid-state material are not very different. In
order to obtain the 60% NPG and 40% PG mixture, a processing step to combine the raw
materials needs to be included in the final cost. This added cost is not reflected in Table 6. The
final cost would still be expected to be on the same order of the encapsulated paraffin. It is
expected cost would be drastically reduced on a large-scale production for both materials.
An advantage paraffin wax has over the solid-state material is in the choice of binder.
Encapsulated paraffin wax can be bonded with quartz chips using a polyester resin, which
significantly reduces the overall cost of the floor tile. Solid-state materials have to use an epoxy
for the binder, which is twice the cost of polyesters.
4.6 Structural Integrity of Encapsulated Particles
Structural integrity is a concern for encapsulated particles. Polyesters often involve an
exothermic cure, which could possibly reach temperatures high enough to degrade the
encapsulation. Encapsulated particles used by Outlast were tested by thermogravimetry analysis
to 300oC without any noticeable damage.
Thermal stability of melamine resin has been shown to be dependent on the curing time and on
several pyrolysis steps. Mass lost during thermogravimetry analysis became smaller with
increased curing times.27 Heat resistance is expected to be enough to tolerate the curing
temperatures of the polyester.
Encapsulated wax particles of a diameter of 5 µm were subjected to the thermal cycling tests by
Yamagishi.48 Tests were performed for a temperature range to allow melting and solidification.
After 5000 cycles, the particles examined under a microscope showed no damage.
Another concern is any damage that may result from the procedure to manufacture the tile.
Currently, the manufacturing process for agglomerate tile using polyester as a binder is
accomplished by mixing the components in a concrete mixer. The mixture is then agitated under
a vacuum to remove air bubbles. It is then heated to induce the curing process. Agitation is not
seen as a risk, but the batch mixing could possibly cause damage. However, the size of the
encapsulated particles compared to the quartz chips is significantly smaller, so damage is
expected to be minimal if any at all. Quartz chips are on the order of several centimeters.
Yamagishi48 performed tests on the structural stability of an encapsulated paraffin particle,
similar to the particles used in the Outlast technology. Encapsulated wax in a brine slurry as a
heat transfer fluid was the focus of the research. The slurry was circulated using a pump system.
Breakage rate was found to increase with increasing circulation times. It was found that the
structural stability of the particle depended on the diameter of the particle. Smaller particles
withstood pressures of a slurry flow and pressure from volumetric expansion. Volumetric
expansion was not a problem due to the flexibility of the shell.
A particle will be broken when the external pressure equals the internal pressure. The internal
pressure in a spherical microencapsulated particle was defined by Yamagishi48 to be related to
the wall tension, thickness and particle diameter.
P = 4 σ t /d
tension of the microencapsulated particle
The particles were also subjected to agitation from a magnetic stirrer. It was found that the
agitation did not damage particles from the size of 5 to 1000 µm.48
Research performed by Roy40 found that the structural strength of particles of wax encapsulated
with polyvinyl alcohol was dependent on the wall thickness. Particles with a wall thickness
comprising 30% of the total particle volume withstood thermal cycling better than particles with
a 15% wall thickness. Particles used by Yamagishi had wall material comprising 14 to 20% of
the total volume. Outlast particles are 20% wall material. The encapsulation material used by
both Yamagishi and Outlast is melamine resin, which is more durable than polyvinyl alcohol.
Outlast uses the encapsulated particles in phase change fabrics for thermal comfort outdoor wear.
Foams are soaked with a solution of the particles. The particles have to be durable enough for
wear and washing in a machine. A concern expressed by Outlast is that high shear stress may
cause damage to the particle. The tile manufacturing process is not expected to exert high shear
stress on the particles.
4.7 Final Material Selection
4.7.1 Phase Change Material
Encapsulated octadecane has been selected as the phase change material. The material will be
supplied by Outlast.
This decision was based on the thermal properties. Octadecane has more than twice the latent
heat storage of the 60%NPG/40%PG mixture. Under cooling effects are significantly less for
octadecane. Currently, the cost of the encapsulated material is the largest drawback of the
octadecane. This cost, however, is expected to decrease with large-scale production.
By selecting encapsulated octadecane, polyester may be used as the binder. Polyester is typically
more than half the cost of epoxies. The encapsulated material should not react adversely with
the binder, as the solid-state phase change material.
Since encapsulated octadecane was selected for the phase change material, a polyester binder can
be used. The polyester resin selected is a styrene-based resin that is used by Granirex. It
requires heating to 80oC to initiate the curing process. A curing agent is also used to aid the
Room temperature and UV cured resins were researched as a possible replacement. The UV
cured resins typically are used for coatings and do not possess the mechanical strength required
for a floor tile application. Suitable room temperature cured resins were not found.
A polyester resin was experimented with that would gel at room temperature, but was still
required to be heated in order to reach full strength. The resin was supplied by Granirex.
4.8 Potential Energy Saving Analysis
Potential energy storage of encapsulated paraffin wax and solid-state phase change materials
have been calculated and presented in Table 3.
4.8.1 Expected Solar Gain
Phase change enhanced floor tile is to be used in a sunspace as additional thermal storage. The
sunspace is assumed to have the appropriate amount of south facing glazing for the maximum
solar gain during the winter months. Assuming Denver, Colorado as the location, the monthlyabsorbed radiation can be determined from the following equation.
1 + cos β
1 − cos β
S = H b Rb (τα ) b + H d (τα ) d
+ Hρ g (τα ) g
monthly average daily beam radiation on a horizontal surface
monthly average daily diffuse radiation on a horizontal surface
monthly average daily radiation on a horizontal surface
average transmittance-absorptance for beam (b), diffuse (d) and
monthly average ratio of beam radiation on a tilted plane to that on
the plane of measurement (usually horizontal)
The collector slope of the south facing glazing has an orientation of 90o. Ground reflectance was
assumed to be 0.3 for each month. Monthly average daily radiation was obtained from weather
data for Denver. Remaining values were calculated using equations from Duffie and Beckman.14
Results are presented in Table 7.
Total monthly radiation incident on the windows of the sunspace, H T , was also calculated and
presented in Table 7. The percentage of the total radiation absorbed into the sunspace is
presented in the last column of Table 7. Calculations were done assuming there was no
overhang above the south facing glazing to shade during the summer. As a result, the absorbed
radiation during the summer months is higher than a typical sunspace with appropriate shading.
Based on the results for the heating months, September through April, the average percentage of
solar radiation that will be absorbed into the sunspace is 70%.
Table 7. Estimated Monthly Absorbed Solar Radition per Area of South Glazing
In order to verify there will be enough radiation absorbed to fully charge the floor tile, the results
from Table 7 and Table 4 have to be multiplied by the appropriate areas. Results from Table 3
and Table 4 are per unit area of the floor, while results from Table 7 are per unit area of south
facing glazing. A floor area of 346.5 ft2 and a glazing area of 352 ft2 were chosen. Based on the
results from Table 8 and Table 9 there is enough absorbed energy per day to fully charge the
floor tiles containing either phase change material at both tile thicknesses.
Table 8. Potential Energy Storage for a Floor Area of 346.5 ft2
Daily Energy Storage
½” Floor Tile
41.2 – 43.8
65.0 – 68.9
Daily Energy Storage
¾” Floor Tile
61.8 – 65.7
97.2 – 103.3
4.8.2 Solar Load Ratio Calculation
It has been determined that there is enough absorbed solar radiation daily to fully charge phase
change materials in floor tile. The next step is to determine the potential savings that can be
achieved with the addition of phase change materials to floor tiles. An empirical method for
estimating the monthly solar and auxiliary energy requirements for passive systems, called the
solar load ratio (SLR), was used for a rough estimate. The monthly solar load ratio is a
dimensionless parameter defined as:
solar energy absorbed per month
building heating load per month
Table 9. Absorbed Average Daily Radiation through South Glazing of Area 352 ft2
Absorbed Solar Radiation
A parameter correlated to the SLR is the solar savings fraction (SSF). It is defined as the
net reference load
The net reference load is the heat loss from the non-solar parts of a building. This includes
walls, floors, ceilings and the roof of everything but the sunspace.
Solar savings is the
difference between the net reference load and the auxiliary heat required by the building.
Net reference load = (NLC) (DD)
Solar Savings = Net Reference Load - Auxiliary Heating Load
net load coefficient
monthly degree day
The net load coefficient is found by summation of the load coefficient of each building element.
Load coefficient is the overall heat transfer coefficient, times the area of the element. The
following definition of NLC was used for this analysis.
NLC = 24 [ (UA)wall + (UA)roof + (UA)glazing + (UA)perimeter + (UA)infiltration ]
(1.1 x (Aglazing/Number of glazing) )
(0.018)(ACH)(ADR)(Volume of building)
Resistance of element
Air changes per hour
Air density ratio
Glazing losses were only considered for the east, west and north facing windows. ADR is
dependent on the elevation of the site. For a building in Denver, Colorado the value is 0.83.
ACH is determined from the design criteria and chosen to be 0.28. Resistance values can be
found from ASHRAE.50
Table 10. Coefficients used for NLC Calculation
(UA) [W / K]
From the solar savings fraction the auxiliary heat required and the solar savings for the building
can be calculated by the following equations.
Auxiliary heat = (NLC) (DD) (1-SSF)
Solar savings = (NLC) (DD) (SSF)
Parameters to determine the above variables have been defined for several reference designs. In
the early eighties, Los Alamos National Laboratories developed reference designs representing
direct gain, trombe walls and sunspace passive systems. A reference design that simulates a
passive system with an attached sunspace was chosen for this analysis. Balcomb2 gives
parameters for several different reference designs. A summary of the major dimensions of the
building is given in Table 11.
The building's heating load was determined by calculating the expected heat loss through the
walls, roof, windows, perimeter and infiltration. Standard values for insulation and infiltration
were used, as defined by ASHRAE.50 Sunspace losses are not considered in this calculation.
Losses from the sunspace are considered in the correlation for the specific reference design.
Balcomb2 has reported these values for the reference designs.
Table 11. Dimensions of Passive Reference Design
Total Volume of Building
Projected area of solar gain
Sunspace floor area
South Facing Glazing Area
Calculations were performed in a spreadsheet. Solar savings were first calculated for the
reference design without any phase change storage. Latent heat storage was included in the
calculation by assuming the heat gained would reduce the heat losses from the building.
Increases in solar savings due to the addition of phase change materials are presented in Table
12. These increases are in addition to savings attained by passive heat gains without latent heat
Table 12. Increase in Solar Savings from Basic Reference Design
Phase Change Material
½” Floor Tile
¾” Floor Tile
Based on the results in Table 12, the addition of latent heat storage does make an impact on the
heating load. As expected, octadecane has the largest increase in savings. Again the calculations
did not include the volume taken by the encapsulation. If the encapsulation material is included,
results of the Kenwax 18 and octadecane would have to be decreased from 85% to 80%.
The solar load ratio is a widely used method since it can be performed either with hand analysis
or simple spreadsheets. Calculations are simplified by the use of reference designs. Annual
results have been reported by Duffie and Beckman14 to be within 3-4% of more detailed
22.214.171.124 Possible Annual Savings
Actual effects of the savings are dependent on the annual heating loads and costs. The size of
the load determines the amount of impact a 10% increase in energy savings has on the annual
heating bill. Lower fuel costs would not see as large as savings as high fuel costs. An analysis
was performed assuming a heating and annual heating load of 50 MBtu at a heating cost of
$11.6/MBtu. Results are presented in Table 13.
It should be noted that the annual heating cost savings presented in Table 13 are only the savings
for adding latent heat storage. Passive savings gained from sensible heat storage have not been
included. The savings, of course, would increase as the heating load increases and as the cost of
Table 13. Annual Heating Cost Savings
Phase Change Material
½” Floor Tile
¾” Floor Tile
4.8.3 Future Simulations
The solar load ratio calculation provided a good estimate of possible savings by the addition of
phase change materials in passive applications. However it does not fully show the effect of
latent heat storage in the floor. It is also a static calculation, where a dynamic simulation would
fully represent the latent heat storage in the floor.
An hourly energy analysis program, the Building Loads Analysis and System Thermodynamics
(BLAST) program, can be used for a dynamic simulation. The program has the ability of
simulating heat transfer and thermodynamics in buildings to characterize the possible energy
savings of using phase change floor tile. BLAST does not explicitly simulate phase change in
building materials such as walls and floor, however specifying layers of high thermal capacitance
can mimic it. Initial simulations have not produced the result expected. Further investigation
into the behavior of the simulation code is required.
Another thermal analysis code, SUNREL, developed by the National Renewable Energy
Laboratory (NREL), simulates phase change in materials. Simulations need to be performed
with the code and compared to the SLR method. Early simulations have yet to produce reliable
4.9 Tile Mixture
The original recipe supplied from Granirex serves as a base for the prototype tile mixture. It is
composed of seven ingredients. A catalyst and wetting agent, silane, are added to the resin
before the other components. The catalyst is 2% the weight of the resin and the silane is 1% of
the weight. Table 14 lists the proportions of the components. The pigment used is carbon black.
Table 14. Granirex Recipe Proportions
Quartz Chips, Mesh 6 (q-6)
Quartz Chips, Mesh 10 (q-10)
Quartz Chips, Mesh 34 (q-34)
Quartz Chips, Mesh 84 (q-84)
Quartz Powder, Mesh 325 (pow)
4.9.1 Varying Binder Proportions
We expected that the mixture of resin and quartz would be the consistency of wet sand before it
was molded and cured. When a mixture was prepared following original recipe, the mixture was
dry. It was quite obvious that there was not enough resin in the mixture. A press was used to
compress the mixture in the tile mold. Approximately 500-1000 psi was applied. Since there
was not enough resin, the compaction was not sufficient. As can be seen in Figure 2, the surface
is not smooth and there are visible gaps.
Figure 2. Sample tile with resin mass fraction of 8% (No phase change material)
By increasing the resin mass fraction from 8% to 12% a mixture with the consistency of wet
sand was achieved. The resulting cured surface is smooth and there are no visible gaps, as
shown in Figure 3.
Figure 3. Sample tile with resin mass fraction of 12% (No phase change material)
The integrity of the cured tile from Figure 2 was not good. Edges of the tile crumbled easily
under light pressure and the components were not compactly compressed. A quick compression
test resulted in the sample crumbling apart under less than 1000 psi of pressure. The tile sample
from Figure 3 had strong edges that did not crumble.
4.9.2 Addition of Phase Change Material
Encapsulated octadecane will be added to the tile mixture by replacing the quartz powder.
Powder is mainly used as filler so it can be replaced by another material, namely the phase
change material. The main goal is to add the phase change material without adversely affecting
the physical properties of the tile.
In order to maximize the amount of phase change material, another component will have to be
replaced in addition to the powder. The q-34 chips will be replaced until the structural integrity
of the tile decreases beyond acceptable limits.
Samples have been made that replaced 100% of the powder that resulted in a successful cure.
However, as with the first samples made with the powder, the resin amount was not enough to
bind the components together properly. Edges crumbled easily and it withstood less than 1000
psi in compressive pressure before crumbling apart. Another problem was encountered with the
addition of the phase change material. The phase change material tended to clump together in
small balls approximately 1/16” in diameter. Several different ways of treating the phase change
material were tried. First the material was dried in a dissector with no added benefit. The
material was then mixed with the resin before the quartz was added. This helped, but clumps
still formed. In Figure 4 the white dots are the clumps of phase change material.
Figure 4. Sample tile with phase change material incorporated with visible clumps.
By running the mixer at a higher speed, the material was fully incorporated. The material was
not dried in a dissector. Figure 5 shows the difference in the surfaces. There are no visible
phase change material clumps.
Figure 5. Sample time with phase change material incorporated without visible clumps.
4.10 Prototype Testing Research
Prototype testing has been separated into two categories, physical and thermal. Physical testing
is important to ensure that the tile is comparable to commercially available agglomerate floor
tile. Thermal analysis will be done to determine the heat storage capability of the tile and to
verify that transition occurs within the appropriate temperature range. The final prototype tile is
not expected to have the highest thermal storage or maximum physical strength, but rather be in
the middle range of thermal and physical properties.
4.10.1 Physical Testing
Prototype tiles will be subjected to physical testing typical of commercially available
agglomerate floor tile. Tests performed by three manufacturers of an agglomerate floor tile
composed of quartz chips and a polyester resin are listed in Appendix 4. Each test performed by
the manufacturer is marked. Physical tests will be selected from this list.
There is overlap in the majority of the tests performed for each type of floor tile which identifies
an industry standard. The tests performed by Granirex are of the most importance since the
recipe for the prototype tile is based on the Granirex recipe. A list of the seven tests that have
been selected for this project are listed in Table 15.
Table 15. Selected Physical Tests
ASTM C-170 Compressive strength
ASTM C-97 Absorption and bulk specific gravity
ASTM C-880 Flexural Strength
ASTM C-484 Thermal Shock
ASTM C-241 Abrasion Resistance
These tests were selected based on the importance of the test to show the physical strength of the
tile. Tests for tile that may be used outdoors were eliminated, such as the freeze thaw and
resistance to de-icing chemicals tests. It is expected that the phase change tile will be for strictly
for indoor usage. Other tests such as smoke density and flame spread were eliminated because
they were not physical strength tests. The tests are also complex and involved and it was felt that
they are unnecessary to perform at this time.
All prototype tiles will undergo acclimation before any testing is performed. Tiles will be held at
a set temperature for a specified amount of time. Humidity will not be controlled. It will be
assumed no change within the time testing will occur. Results from the tests will be compared to
the results obtained from Granirex, and to a standard tested along with the prototypes. The
standard will be a piece of floor tile obtained from Granirex.
126.96.36.199 Initial Testing
The listed tests in Table 15 do not have to be performed on each prototype tile. This would be
time consuming and a needless use of materials. Results from a select group of tests will be
significant to eliminate a majority of the prototype tiles. Once the first elimination is made, the
remaining tests can be performed. Two tests have been selected for the initial round of testing.
These are compressive strength and 3-point flexural tests. They were selected based on the
information they would provide on the strength of the tile and the ease of performing the test.
A morphology analysis will also be performed on a tile with and without phase change material.
This is important to fully understand the behavior of dispersion of the phase change material
through the mixture. It will also help to verify whether or not the phase change material is
4.10.2 Thermal Testing
Testing performed with a differential scanning calorimeter (DSC) requires samples in the order
of milligrams. These can be obtained either by drilling samples from prototype tiles that have
cured, or allowing samples to cure in the pans used for DSC analysis. Both procedures involve
inconstancies and are dependent on the homogeneity of the batch. Samples can be taken from
regions with very little phase change material, showing results that may not be accurate.
However multiple samples from a batch should help to eliminate some of the uncertainty.
Another possible testing technique would be to test the entire prototype tile. This requires an
apparatus that is capable of providing a constant heat flux. The temperature can then be
monitored throughout the temperature range watching for indication of a phase change.
Test samples will be batches cured in the sample DSC pan. At least five DSC samples will be
made from each batch. More extensive thermal testing can be performed after the first
elimination. This would involve testing an entire tile. If this procedure does not give reliable
results, samples will be taken from the prototype tiles.
5. PROTOTYPE MANUFACTURE
Prototype tiles have been manufactured with varying amounts of resin and phase change
materials. All tiles are made with a four-inch square mold shown in Figure 6. The mixture is
added to the mold and pressed under 500-1000 psi of pressure. Figure 7 shows the mold in the
press. While the mixture is still in the mold it is heated to approximately 85oC for twenty
minutes. After twenty minutes the tile is removed and the curing process is finished in an oven
set to 100oC for approximately four hours. This second cure in the oven is done to ensure that all
the resin has cured. One method of determining this state is the lack of polyester odor from the
Figure 6. 4" Tile Mold
The tile mixture is combined together in a kitchen mixer. Catalyst and the wetting agent are
added to the resin and these are mixed for 30 seconds. Quartz chips are then added and mixed
for another minute. Next, quartz powder is incorporated into the mixture slowly. Once all the
powder is added to the mixture it is mixed for another two minutes. Tiles have completed the
curing process after resting for 24 hours at room temperature after curing in the oven. At this
point the tiles can be cut in the appropriate sizes for testing. A wet-saw with a diamond blade is
used to cut the tiles.
Figure 7. Tile mold in the press.
6. RESULTS AND DISCUSSION
Performance of the tiles will be based on the results of both physical and thermal tests. Physical
tests are important in order to have a comparison to like tiles on the market. Thermal tests are
needed to verify that the tile is storing latent heat and that the phase change is happening at the
6.1 Preliminary Compression Testing
The compression test was performed on a set of initial samples since it was easy to perform and
gave a good metric on the bonding strength of the resin. It became apparent that there was not
enough resin in the mixture. The tiles all crumbled under 1000 psi of pressure. Expected
strength of the tiles was 25,000 psi. Based on the results of those tested, it was decided to
increase the amount of resin in the mixture. This is not a concern, as resin percentage in the
mixture is not fixed. The amount of resins required can be sensitive to humidity and the
container used for mixing. It will wet the container, which leads to less resin being incorporated
into the mixture.
By increasing the resin mass fraction from 8% to 12%, a much wetter mixture was obtained.
This resulted in a properly compacted and cured tile. Several other samples were made with
resin amounts varying between 8% and 12%. These samples need to undergo a round of
compression testing to determine a mixture with the minimum amount of resin that does not
reduce the structural integrity.
Next, samples were made that included the phase change material. The quartz powder was
replaced with the phase change material in the mixture. In order to overcome the dispersing
problem, the mixture was mixed at a higher speed and for a longer period of time. This resulted
in the material being dispersed throughout the mixture.
6.2 Preliminary Thermal Testing Results
Samples were taken from mixtures with and without phase change materials and cured in a DSC
pan. The result from the heating run of a test is given in Table 16.
Table 16. Preliminary DSC Testing
Peak Transition Temperature
Expected Results 31.2oC
Based on these initial results, the incorporated phase change material is undergoing a phase
change at the appropriate temperature. The latent heat is also on the order of expected values.
When similar runs were performed with solid-state phase change materials, the latent heat was
significantly reduced from expected values due to an adverse reaction with the epoxy.
Early evaluation of the potential energy storage of phase change materials in floor tile for passive
solar applications have been promising. Using encapsulated octadecane in a 3/4" thick floor tile,
annual heating savings can be increased by 24%. Solid-state phase change material has possible
energy savings of half that amount. It was therefore concluded octadecane would be the best
material for this application. The analysis done to date has been for a static model and the results
are expected to be a low estimate of the possible energy savings. A dynamic analysis may
provide more realistic results and higher savings.
Each prototype tile will contain quartz chips and powder, polyester resin and encapsulated
paraffin wax. Tiles will be made with varying amounts of quartz powder, encapsulated wax and
resin. The amount of quartz chips will be held constant to ensure structural integrity of the tile.
Resin will be varied from 5% to 10% of the total mixture. Proportions of encapsulated wax and
quartz powder will be directly dependent on each other. The ideal case would be a tile
containing all phase change material and no quartz powder.
Ten design points, each containing different amounts of resin, quartz powder and encapsulated
wax were identified. Prototype tiles will be manufactured at each of these points. Two to four
batches will be made for each design point depending on the size and number of prototype tiles
required. The materials will be supplied by the companies, Granirex and Outlast Technology.
Manufacture of the prototype tile will be done in labs at Colorado State University (CSU).
Prototype tiles will be subjected to both physical and thermal testing. Samples will be made to
the size recommended by the test standards.
Physical tests have been broken down into two phases, initial and final. This significantly
reduces the number of prototype tiles that need to be manufactured. Results from the initial
phase of testing will be used to select two or three of the best performers. These selected tiles
will then be subjected to the final round of testing. A majority of the tests will be performed at
CSU, although two or three of the tests will have to be out-sourced.
Eighty-prototype tiles have to be made for the initial phase of testing. Seventy-six have to be
manufactured for the final round of testing if two are selected after the initial testing phase.
Thermal testing will occur during the initial phase of testing. Samples will be cured in the DSC
pans and subjected to analysis. At least five samples will be made from each batch at each
Based on the results of the thermal and physical tests, the best proportion of phase change
material in a tile will be selected. This will be accomplished by a statistical analysis of the
testing results. The potential annual savings can be calculated for this proportion of phase
change material. It can then be determined if the cost savings are worth the initial investment of
installing the floor tile.
1. Arndt, P.E. , Dunn, J.G., Swillix, R.L., “Organic Compounds as Candidate Phase Change
Materials in Thermal Energy Storage”, Thermochimica Acta, Vol. 79, pp. 55-68, 1984
2. Balcomb, D., Passive Solar Heating Analysis, American Society of Heating, Refrigerating
and Air-Conditioning Engineers, Atlanta, 1984
3. Barrio, M., Font, J., Muntasell, J., Tamarit, J., “Floor Radiant System with Heat Storage by a
Solid-State Phase Transition Material”, Solar Energy Materials and Solar Cells, Vol. 27, pp.
4. Benson, D.K., Chandra, D., “Solid-State Phase Change Materials for Thermal Energy
Storage”, Electrochemical Society Extended Abstracts, Vol. 85-2, 1985
5. Benson, D.K., Christensen, C.B., Burrows, R.W., Sinton, Y.D., “New Phase-Change
Thermal Energy Storage Materials for Buildings”, Enerstock 85, III International Conference
on Energy Storage for Building Heating and Cooling, 1985
6. Benson, D.K., Webb, J.D, Burrows, R.W, McFadden, J.D., Christensen, C., “Material
Research for Passive Solar Systems: Solid State Phase Change Materials”, SERI Report TR255-828, 1985
7. Benson, D.K., Webb, J.D, Burrows, R.W, McFadden, J.D., Christensen, C., “Material
Research for Passive Systems: Solid State Phase Change Material and Polymer
Photodegradation”, Passive and Hybrid Solar Energy Update, 1982
8. Brostow, W., “An Introduction to Liquid Crystallinity” in Liquid Crystal Polymers: From
Structures to Applications, (Eds. A.A. Collyer), Elsevier Applied Science, London, 1992
9. Busico, V. Carfagna, C., Salerno, V., Vacatello, M., “The Layer Perovskites as Thermal
Energy Storage System”, Solar Energy, Vol. 24, pp. 575-579, 1980
10. Chandra, D., Jorgensen, G., “The Structure and Lattice Parameters of Pentaerythritol Above
and Below its Phase Transition Temperature”, Advances in X-ray Analysis, Vol. 28, 1985
11. Colvin, D.P., Mulligan, J.C., Bryant, Y.G., "Enhanced Heat Transport in Environmental
Systems Using Microencapsulated Phase Change Materials", Report 921224
12. Cornell, John A., Experiments with Mixtures, John Wiley & Sons, New York, 1990
13. “Differential Scanning Calorimetry”, Macrogalleria, University of Southern Mississippi
Department of Polymer Science, 01 Jan. 1999, <http://www.psrc.usm.edu/macrog>
14. Duffie, John A., Beckman, William A., Solar Engineering Of Thermal Processes, John Wiley
and Sons, New York, 1991
15. "EPI-CURE 3140", Shell Chemicals - Online Literature, 1 Oct. 1999, <http://www.resinsversatics.com/rsins>
16. "Epon Resin 828", Shell Chemicals - Online Literature, 1 Oct. 1999, <http://www.resinsversatics.com/rsins>
17. Feldman, D., Banu, D., Hawes, D.W., "Development and application of organica phase
change mixtures in thermal storage gypsum wallboard", Solar Energy Materials and Solar
Cells, Vol. 36, pp. 147-157, 1995
18. Font, J., Muntasell, J., Cardoner, F., “Preliminary Study of a Heat Storage Unit Using a
Solid-Solid Transition”, Solar Energy Materials and Solar Cells, Vol. 33, pp. 169-176, 1994
19. Font, J., Lopez, D., Muntasell, J., “Low Temperature Invariant in Pentaerythritol/Neopentyl
Glycol Binary System”, Material Research Bulletin, Vol. 24, pp. 1251-1259, 1989
20. Font, J., Muntasell, J., Navarro, J., Tamarit, J., “Melanges Pentaglycerine/Neopentyl Glycol :
Formation d’une Solution Solide”, Thermochimica Acta, Vol. 136, pp. 55-71, 1988
21. Font, J., Muntasell, J., Navarro, J., Tamarit, J., “Calorimetric Study of the Mixtures PE/NPG
and PG/NPG”, Solar Energy Materials, Vol. 15, pp. 299-310, 1987
22. Font, J., Muntasell, J., Navarro, J., Tamarit, J., “Time and Temperature Dependence of the
Exchanged Energy on Solid-Solid Transitions of Pentaglycerine/Neopentyl Glycol
Mixtures”, Solar Energy Materials, Vol. 15, pp. 403-412, 1987
23. Gray, G.W., Windsor, P.A., Liquid Crystals and Plastic Crystals Vol I, Haslted Press, New
24. Hawes, D.W., Feldman, D., Banu, D., "Latent heat storage in building materials", Energy and
Buildings, Vol. 20, pp. 77-86, 1993
25. Himran, S., Suwone, A., Mansoori, G., “Characterization of Alkanes and Paraffin Waxes for
Application as Phase Change Enery Storage Medium”, Energy Sources, Vol. 16, pp. 117128, 1994
26. Hinkelmann, K., Kempthorne, O., Design and Analysis of Experiments: Volume I
Introducion to Experimental Design, John Wiley & Sons, New York, 1994
27. Hirata, Toshimi, "Melamine Resin (Pyrolysis)" in Encyclopedia of Polymer Science and
Engineering Volume 7, John Wiley and Sons, New York 1987
28. Hull, D., Clyne, T.W., An Introduction to Composite Materials, (Eds. D.R. Clarke, S. Suresh,
I.M. Ward), University Press, Cambridge, 1996
29. Johnson, Timothy E., "MIT Solar Building N0. 5: The Third year Performance", Passive
Solar Journal, Vol. 1, No. 3, 1982
30. Johnson, Timothy E., “The MIT Crystal Pavilion”, Progress in Passive Solar Energy
Systems, pp. 255-260, 1982
31. Kedl, R.J., “Conventional Wallboard with Latent Heat Storage for Passive Solar
Applications”, Proceedings of the InterSociety Energy Conversion Engineering Conference,
Aug 12-17, Vol. 4, pp 222-225, 1990
32. Lee, H., Neville, K., Handbook of Epoxy Resins, McGraw Hill, New York, 1967
33. Magill, Monte, "An Overview of the Outlast Temperature Regulation Technology", 23 Jun.
34. Morton, D.H, Polymer Processing, Chapman and Hall, London, 1989
35. Moscicki, J.K., “Dielectric Relaxation in Macromolecular Liquid Crystals” in Liquid Crystal
Polymers: From Structures to Applications, (Eds. A.A. Collyer), Elsevier Applied Science,
36. Mulligan, J.C., Colvin, D.P., Bryant, Y.G., "Microcapsulated Phase Change Material
Suspensions for Heat Transfer in Spacecraft Thermal Systems", Journal of Spacecraft and
Rockets, Vol. 33, No. 2, 1996
37. Naumann, R., Emons, H., “Results of Thermal Analysis for Investigation of Salt Hydrates as
Latent Heat-Storage Materials”, Journal of Thermal Analysis”, Vol. 35, pp. 1009-1031, 1989
38. Neeper, D.A., “Potential Benefits of Distributed PCM Thermal Storage”, Prepared by
Advanced Engineering Technology Group at Los Alamos National Laboratory
39. Potter, W.G., Uses of Epoxy Resins, Newnes-Butterworths, London, 1975
40. Roy, Sanjay, Sengupta, S., "An Evaluation of Phase Change Microcapsules for use in
Enhanced Heat Transfer Fluids", International Communications in Heat and Mass Transfer,
Vol. 18, pp. 495-507, 1991
41. Salyer, Ival O., Sircar, Anil K., Kumar, Alok, “Advanced Phase Change Materials
Technology: Evaluation in Lightweight Solite Hollow-Core Building Blocks”, Proceedings
of the InterSociety Energy Conversion Engineering Conference, Jul 30 – Aug 4, Vol. 2, pp.
42. Salyer, I.O., Sircar, A.K., “A review of phase change materials research for thermal energy
storage in heating and cooling applications at the University of Dayton from 1982 to 1996”,
International Journal of Global Energy Issues, Vol. 9, No. 3, pp. 183-198, 1997
43. Solomon, A.D., “Latent Heat Thermal Energy Storage and Waste Heat Reuse in a Single
Periodic Kiln”, Proceedings of the InterSociety Energy Conversion Engineering Conference,
Aug 12-17, Vol. 4, pp 226-229, 1990
44. Sözen, M., Vafai, K., Kennedy, L., "Thermal Charging and Discharging of Sensible and
Latent Heat Storage Packed Beds", Journal of Thermophysics and Heat Transfer", Vol.5,
45. Timmermans, J., “Plastic Crystals: A Historical Review”, Journal of Physics, Chemistry and
Solids, Vol. 18, No. 1, pp. 1-18, 1961
46. Thorncroft, G.E., Gunnerson, F.S., “Performance Evaluation of a Solid State Phase Change
Material for Thermal Storage Applications”, Intersociety Energy Conversion Engineering
47. Tomlinson, John J., Heberie, David D., “Analysis of Wallboard Containing a Phase Change
Material”, Proceedings of the InterSociety Energy Conversion Engineering Conference, Aug
12-17, Vol. 4, pp 230-235, 1990
48. Yamagishi, Y., Sugero, T., Ishige, T., Pyateriko, A., "An Evaluation of Microcapsulated
PCM for Use in Cold Energy Transportation Medium", Proceedings of the 31st Intersociety
Energy Conversion Engineering Conference, Washington D.C, Aug 11-16, Vol. 3, 1996
49. Yamagushi, M., Sayama, S., "Heat Storage-Type Floor Heating System with Heat Pump
Driven by Nighttime Electric Power", Heat Transfer-Japanese research, Vol. 26, No. 2, pp.
50. 1993 ASHRAE Handbook of Fundamentals, Atlanta, American Society of Heating,
Refrigeration and Air-Conditioning Engineers, Inc, 1993
9. APPENDIX 1
Solid-State Phase Change Materials
Figure 8. Molecular structure of pentaerythritol, C – (CH2OH)4
Figure 9. Molecular structure of pentaglycerine, (CH3) – C – (CH2OH)3
Figure 10. Molecular structure of neopentyl glycol, (CH3)2 – C – (CH2OH)2
Latent Heat [kJ/kg]
Figure 11. Latent Heat for Binary Mixture of Neopentyl Glycol and Pentaglycerine
Kenwax 18 Normal Paraffin Content
Table 17. Kenwax 18 Paraffin Content
Normal Paraffin Content
Kenwax 19 Normal Paraffin Content
Table 18. Kenwax 19 Paraffin Content
Normal Paraffin Wax
11. APPENDIX 3
Figure 12. Molecular Structure of Melamine-Formaldehyde
12. APPENDIX 4
Table 19. Physical Tests Performed on Agglomerate Floor Tile by Various Manufacturers
Verona Marble Co.
ASTM C-615 Granite Dimension Stone
ASTM C-97 Absorption and bulk specific
ASTM C-170 Compressive strength
ASTM C-648 Breaking Strength
ASTM C-880 Flexural Strength
ASTM C-484 Thermal Shock
ASTM C-531 Thermal Coefficient of
ASTM C-1026 Frost Resistance
ASTM C-501 Relative Resistance to Wear
ASTM C-241 Abrasion Resistance
ASTM C-1028 Coefficient of Friction
ASTM D-2299 Stain Resistance
ASTM C-672 Resistance to De-Icing
ASTM G-23 Ultra Violet Performance
ASTM E-84 Flame Spread
ASTM E-662 Smoke Density
ASTM C-99 Modulus of Rupture
ASTM C-307 Tensile Strength
ASTM D-695 Compression Strength
ASTM D-1042 Dimensional Stability
ASTM D-2583 Indentation Hardness
ASTM D-2047 Coefficient of Friction
ASTM D-54384 Stain Resistance
ASTM C-291 Wear Resistance/Hardness
ANSI A-137.1 Ceramic Standard
NES 713-1985 Mean Toxicity Index